Mat.No. 1.5864, DIN 35NiCr18
Designation by Standards Brand Name Ravne No. Mat. No. DIN EN AISI VCN45 757 1.5864 35NiCr18 - - Chemical Composition (in weight %) C Si Mn Cr Mo Ni V W Others 0.35 0.25 0.60 1.30 - 4.50 - - - DescriptionAlloyed carbon steel. ApplicationsGears, driving shafts, shafts, wheels. Physical properties (avarage values) at ambient temperatureModulus of elasticity [103 x N/mm2]: 210 Density [g/cm3]: 7.85 Soft AnnealingHeat to 580-610oC, cool slowly. NormalizingTemperature: 83...
Designation by Standards
|Brand Name||Ravne No.||Mat. No.||DIN||EN||AISI|
Chemical Composition (in weight %)
Alloyed carbon steel.
Gears, driving shafts, shafts, wheels.
Physical properties (avarage values) at ambient temperature
Modulus of elasticity [103 x N/mm2]: 210
Density [g/cm3]: 7.85
Heat to 580-610oC, cool slowly.
Harden from a temperature of 820-850oC followed by oil or air quenching.
Tempering temperature: 450-650oC.
Hot forming temperature: 1100-850oC.
Forms manufactured: Please see the Dimensional Sales Program.
The information and data presented herein are typical or average values and are not a guarantee of maximum or minimum values. Applications specifically suggested for material described herein are made solely for the purpose of illustration to enable the reader to make his own evaluation and are not intended as warranties, either express or implied, of fitness for these or other puposes. There is no representation that the recipient of this literature will receive updated editions as the become available.